Int. J. Electrochem. Sci., 13 (2018) 9399 – 9415, doi: 10.20964/2018.10.39
International Journal of
The Effect of Heat Treatment on the Corrosion Resistance,
Mechanical Properties and Wear Resistance of Cr−C Coatings
Composite Coatings Electrodeposited on Low
Hung-Hua Sheu1,*, Ting-Yi Hong1, Tzu-Te Lin2, Ming-Der Ger1*
Department of Chemical and Materials Engineering, Chung Cheng Institute of Technology, National Defense University, Taoyuan City, Taiwan
Department of Power Vehicle and Systems Engineering, Chung Cheng Institute of Technology, National Defense University, Taoyuan City, Taiwan
*E-mail: email@example.com, firstname.lastname@example.org
Received: 5 June 2018 / Accepted: 30 July 2018 / Published: 1 September 2018
In order to enhance the corrosion resistance, mechanical properties and wear resistance of Cr−C thin films, Cr−C/Al2O3 composite coating is electrodeposited from the Cr(III) plating bath containing
Al2O3 particles in this study. The Cr−C/Al2O3 composite coating has the best corrosion resistance
which icorr is approximately at 2.84 × 10-7 A/dm2, but the corrosion resistance will reduce with an
increase of heating temperature due to the formation of cracks within Cr−C/Al2O3 composite coatings.
The effect of heat treatment on the mechanical properties and tribological behavior of Cr−C coating and Cr−C/Al2O3 composite coating is examined. The experimental results show that the hardness of
Cr−C coating and Cr−C/Al2O3 composite coating increased with a heat treatment process due to the
precipitation of chromium carbide and chromium oxide. The incorporation of Al2O3 particles into the
Cr−C matrix can significantly enhance the micro-hardness and reduce the wear rate of Cr−C/Al2O3
composite coating as compared to that of Cr−C coating. The highest micro-hardness of Cr−C/Al2O3
composite coatings (22.85 GPa) is achieved after the coatings heated at 600 ℃. The co-deposition of Al2O3 particles within the Cr−C deposits will significantly improve the wear resistance of coatings and
reduces the wear weight loss. The lowest specific wear rate (8.8 × 10-7 mm3/Nm) was obtained for the Cr−C/Al2O3 composite coatings heat treated at 200 ℃.
Keywords: Cr−C/Al2O3 composite coating, wear rate, Cr(III) bath, heat treatment 1. INTRODUCTION
than 10 μm  and cracks are frequently observed  for the Cr coatings electroplated from the trivalent chromium baths, which are detrimental to their wear and corrosion properties. A metal matrix composite is a good way to gain a greater wear and corrosion properties.
Ceramic particles-reinforced composite coatings have been widely developed due to their high hardness, good wear and corrosion resistance compared to pure metal or alloy coatings. Electroplating is one of the suitable methods for producing the composite coatings by co-deposition of inert particles into a metal matrix. These improved properties mainly depend on the content and nature of particles in the coatings. These inert particles including SiC, Al2O3, WC, TiO2, Si3N4, and diamond [10-16] are
frequently co-deposited into metal matrices to form composite coatings. Among these particles, alumina (Al2O3) has many superior properties, such as low price, good chemical stability, high
hardness, and wear resistance at high-temperature . Therefore, as a second phase to strength composite materials, Al2O3 is one of the economic and powerful materials. It has been shown that
modification of mechanical and electrochemical properties, including increased resistance to wear, increased corrosion resistance, and increased hardness could be achieved by incorporation of hard Al2O3 particles in chromium coatings [18-20].
On the other hand, it is well known that heat treatment will cause changes in microstructures of metals such as phase change, grain size, residual stress and crack, leading to the enhancement of hardness of the coatings [21-23]. Annealing at elevated temperatures has also been utilized to improve the mechanical properties of the trivalent chromium coatings. The literatures had found that with an annealing of the trivalent chromium coatings, the hardness of Cr–C coating increases due to the crystallization of chromium and precipitation of hard chromium carbides phases [2, 24]. In our previous study , heat treatment was utilized to improve hardness of the Cr−C-Al2O3 composite
coating. The hardness increases with heat treatment temperature. The highest hardness (HV 1520) was found for Cr−C-Al2O3 composite coating annealed at 600 °C due to the precipitation of Cr23C6 and
Cr2O3 during the treatment, whereas heat treatment at 600 °C had an inverse effect on the corrosion
resistance. The possible explanation was that the precipitation of chromium carbides would increase the residual stress caused by a serious lattice distortion and form great amount of cracks within Cr−C coatings, leading to the corrosion resistance decreased after annealing at 600 °C. However, the effect of heat treatment on anti-wear behavior of trivalent Cr−C/Al2O3 coatings is seldom studied. Therefore,
in this work, the hardness values and wear resistance of as-plated, annealed Cr–C alloy deposits and annealed Cr–C/Al2O3 composite deposits are discussed.
ammonium formate as complexing agent, 0.02 M KBr, 0.6 M KCl and 0.5 M B(OH)3. The
Cr−C-Al2O3 composite coatings were prepared by adding 15 g/L Al2O3 particles with an average diameter of
0.3 µm into the plating bath. Magnetic stirring and subsequently by ultrasonic agitation for 40 min just prior to electroplating were utilized to make the dispersion of Al2O3 particles become uniformly. The
electroplating was carried out for 1 h with the conditions of pH 4.5, temperature of 25 °C, stirring rate of 300 rpm, and current density of 20 A/dm2. The as-deposited Cr−C alloy coatings and Cr−C-Al2O3
composite coatings were heat treated in an oven filled with nitrogen atmosphere at temperatures of 200, 400 and 600 °C, respectively, for 1 h.
The surface and cross-section morphologies of Cr–C and Cr–C–Al2O3 deposited specimens
were examined with a field emission scanning electron microscopy (FESEM, HITACHI S-3000 N, operating at 15 kV). The crystalline structure and constituent phase of the coatings were examined by a X-ray diffraction (XRD, BRUKER D2 PHASE) with Cu Kα radiation (λ = 0.15405 nm) over a
scanning range from 10° to 100°. A differential scanning calorimeter (DSC, NETZSCH DSC 404F3) was used to detect the thermal events with a heating rate of 20 °C/min from room temperature up to 700 °C.
The potentiodynamic polarization tests were carried out in a standard three-electrode cell system using an Autolab-PGSTAT30 potentiostat/galvanostat controlled by a GPES (General Purpose Electrochemical system) software and stabilized at open circuit potential (OCP) before electrochemical test. A platinum sheet and Ag/AgCl electrode were used as the counter and reference electrodes, the linear polarization curves of Cr-C and Cr–C/Al2O3 composite coatings were measured after 20 min
immersion of specimens in a 3.5% NaCl aqueous solution at room temperature in the potential range between -0.3 V and 0.5 V with a scanning rate of 0.5 mV s-1.
A Nano-Indenter XP system (NIS) made by MTS Co. Ltd. was used to measure the hardness of the films. All samples were indented with an applied load of 2500 µN. For each sample, the hardness considered is an average value of five measurements conducted at various locations. The average hardness was given directly by the NIS system. In order to ensure the absence of thermal drift, a 10 s pause time was given between loading and unloading cycles.
A ball-on-disk tribometer (SENSE-7) was employed to measure the tribological properties of the coatings. The commercially obtained steel balls (ψ6.25 mm) were used as the counterpart. The friction tests were carried out at a reciprocating sliding velocity of 4 m/s under a load 6 N for a distance of 60 m, and the sliding stroke was around 1.00 mm. Each of these tests was repeated three times. All the experiments were accomplished in ambient condition of temperature 25±1 °C and 50%±2% relative humidity. No lubrication was used during wear tests. The volumetric wear rate (Rw) of specimens was calculated by Rw = V/F•S, where V is the wear volume (mm3), F is the applied load (N), and S is the sliding distance (m). The wear volume was obtained by a non-contact surface mapping profiler (ADE Corporation, USA).
The SEM morphologies of the as-deposited and heat treated Cr−C coatings are displayed in Fig. 1. The as-deposited sample presents a typical nodular structure with some microcracks (red arrows in Fig. 1(a)) on the coating. It is believed that the reduction of hydrogen ions during the electrodeposition process results in hydrogen evolution and crack formation. In the case of Cr−C deposit annealed at 200 °C, an increase in the number of cracks in the Cr−C coating (red arrows in Fig. 1(b)) can be observed. A network structure of cracks all over the Cr−C coatings annealed at 400 °C and 600 °C is formed and the cracks become much wider and broader compared to the one annealed at 200 °C (Fig. 1(c) and (d)), The hardness of Cr−C coatings will be significantly enhanced due to the precipitation of Cr23C7, and Cr7C3 during heating [25,26]. In general, the enhanced hardness of metal
materials also will decrease the toughness of metals (or enhance its brittleness), leading to the reduction in fracture toughness and yield stress .
Figure 1. SEM surface morphologies of Cr−C coatings heated at various temperatures: (a) as-plated, (b) 200 ℃, (c) 400 ℃ and (d) 600 ℃.
Consequently, the materials with a high hardness will be fractured easily by various stresses such as thermal stress, residual stress and impact stress etc. Therefore, one possible explanation for the increase of microcrack density by annealing is due to the release of internal (residual) stress . In addition, owing to the different thermal expansion coefficients between steel substrates (about 13 × 10
treatment, resulting in the formation of the cracks. However, the change of phase structure from amorphous to crystalline might also has some influence on it.
Fig. 2 shows the morphologies of the as deposited and heat treated Cr−C/Al2O3 composite
coatings. It shows from Fig. 2(a) that no cracks are seen on the as deposited Cr−C/Al2O3 composite
coating. On annealing Cr−C/Al2O3 coating at 200 °C the crack free microstructure is maintained (Fig.
2(b)). At higher annealing temperatures of 400 °C and 600 °C (Fig. 2(c) and 2(d)), a network of cracks occurs and the density of cracks network within Cr−C/Al2O3 composite coatings becomes less dense as
the heat treatment temperature increasing. The obvious network of cracks appears in Cr−C/Al2O3
composite coatings heated at higher temperature can be mainly attributed to the effect of thermal stress. It shows from Fig. 2(b) that the, this indicates the added Al2O3 particles can reduce the internal
(residual) stress of coatings during electroplating process and this result is also in agreement with our previous study . Fig. 3 presents SEM cross-sectional images for the as-plated coatings of Cr−C coatings and Cr−C/Al2O3 composite coating, respectively.
Figure 2. Surface morphologies Cr–C/Al2O3 composite deposit heated at various temperatures: (a)
as-plated, (b) 200 ℃, (c) 400 ℃ and (d) 600 ℃.
structure took place within Cr−C/Al2O3 composite coating due to incorporation of these dispersion
Al2O3 particles into the Cr−C deposit leads to the reduction of the coating internal stresses .
Figure 3. SEM cross-sectional images of the as-plated coatings: (a) Cr–C coating, (b) Cr–C/Al2O3
Figure 4. DSC curve of the as-plated Cr−C coating tested in a flowing nitrogen atmosphere and with a heating rate of 20 ℃min−1.
Figure 5. The X-ray diffraction patterns of Cr−C coatings after annealing at different temperatures: (a) as-plated, (b) annealed at 200 ℃, (c) annealed at 400 ℃, and (d) annealed at 600 ℃.
Figure 6. The X-ray diffraction patterns of Cr−C/Al2O3 composite coatings after annealing at different
are shown in Fig. 5. Fig. 5(a) shows that the as deposited Cr−C coating is amorphous. As shown in Fig. 5(b), a sharp peak exists together with the broad peak around at 2θ = 43.5° was observed for the Cr−C coating annealed at 200 ℃, indicating the Cr–C coating starts to crystallize at temperatures lower than 200 ℃. However, the crystallization is not completed until 400 ℃. Fig. 5(c) presents that the appearance of Cr and Cr23C6 peaks after the Cr−C coatings heating at 400 ℃. When the Cr−C
coatings are heated at 600 ℃, the diffraction peaks indicated Cr, Cr23C6, Cr7C3 and Cr2O3 appear in the
XRD pattern (Fig. 5(d)). The above results are in agreement with previous studies that the Cr−C coatings heated at 600 ℃ will precipitate Cr23C6 and Cr7C3 phases and enhance the hardness of
By comparing Fig. 4 and Fig.5, we can conclude that the exothermic peak “P1” in the range from 100 to 180 ℃ is related to the partial crystallization of chromium within Cr−C coating, peak “P2” in the range from 280 to 400 ℃ can be attributed to the formation of Cr23C6 phase and
re-crystallization of Cr, peak “P3” in the range from 560 to 620 ℃ should be the formation of Cr7C3 and
Cr2O3. The Cr−C/Al2O3 composite coatings present a similar XRD pattern with that of Cr−C coating,
both in as plated and heat-treated conditions (Fig. 6). The X-ray diffraction angles occurred at 25.5°, 35.3° and 58° indicate the existence of Al2O3 particles within Cr−C matrix.
Figure 7. Potentiodynamic polarization curves of Cr-C coatings and Cr−C/Al2O3 composite coatings:
(a) as-plated Cr-C coatings and Cr−C/Al2O3 composite coatings, (b) Cr-C coatings with heat
Fig. 7 shows the potentiodynamic polarization curves of the as-plated Cr-C coatings, as-plated Cr−C/Al2O3 composite coating and the coatings heated at various temperature. The corrosion
potentials (Ecorr), corrosion current densities (icorr) , anodic and cathodic Tafel slopes (βa and βc)
derived from the potentiodynamic polarization curves of steel substrates, as-plated coatings and coatings after heating at different temperature were also presented in Table 1.
Table 1. Corrosion characteristics of Cr−C coatings and Cr−C/Al2O3 composite coatings heated at
various temperature measured from 3.5 wt.% NaCl solution.
Sample code βa (V/ decade) βc (V/ decade) icorr (A/dm2) Ecorr (V vs. SEC)
Steel substrates 0.215 -0.305 4.83×10-5 -0.41
As-plated Cr−C coatings 0.267 -0.364 1.31×10-6 -0.80
Cr−C coatings heated at
200℃ 0.254 -0.355 2.34×10-6 -0.69
Cr−C coatings heated at
400℃ 0.238 -0.378 6.56×10-6 -0.52
Cr−C coatings heated at
600℃ 0.226 -0.381 2.19×10-5 -0.52
composite coatings 0.283 -0.375 2.84 × 10
-0.50 Cr−C/Al2O3 composite
coatings heated at 200℃ 0.256 -0.368 5.42 × 10-7 -0.62
coatings heated at 400℃ 0.238 -0.346 8.62 × 10-7 -0.58
Figure 8. Loading-unloading curves of various coatings after annealing at different temperatures: (a) Cr−C coatings, (b) Cr−C/Al2O3 composite coatings.
Fig. 7(a) presents both Cr-C coatings and Cr−C/Al2O3 composite coatings has excellent
corrosion resistance than that of steel substrates, and their icorr is approximately at 1.31 × 10-6 and 2.84 × 10-7 A/dm2, respectively. It also can see that the corrosion resistance of Cr−C/Al2O3 composite
coatings is better than that of Cr-C coatings, it can be attributed to the Cr−C/Al2O3 composite coatings
has a cracks-free structure (see Fig. 1(a) and Fig. 2(a)) that can obstruct the corrosion factors to corrode the substrates along the cracks within coatings. In Table 1, the icorr of Cr-C coatings decrease
with the increasing of heat temperature from 1.31×10-6 A/dm2 to 2.19×10-5 A/dm2. The same condition also occurred at Cr−C/Al2O3 composite coatings, but the Cr−C/Al2O3 composite coatings still maintain
an excellent anti-corrosion behavior (2.84 × 10-7 to 8.62 × 10-7 A/dm2) until heated at 400℃, the icorr
also still keep at 4.11×10-6 A/dm2 after heating at 600℃. The corrosion resistance of Cr−C/Al2O3
composite coatings are significantly better than that of Cr-C coatings after heat treatment, due to the added Al2O3 particles will reduce the internal stress of Cr-C matrix  and inhibit the formation of
cracks within Cr-C matrix during heating process.
Nano-indentation test can reflect the hardness of materials  and the elastic modulus of the thin films is an important mechanical property of the coatings . Besides, hardness and elastic modulus can be affected by various factors such as microstructure and heat treatment . To evaluate the mechanical properties of Cr−C coatings and Cr−C/Al2O3 composite coatings after heat treatment,
the micro-hardness of various coatings are performed by nano-indentation tests. The typical displacement-load curves of the Cr−C coatings and Cr−C/Al2O3 composite coatings are shown in Fig.
Figure 9. Effect of annealing temperature on the hardness of Cr−C coating and Cr−C/Al2O3 composite
Figure 10. SEM morphologies of the worn surfaces of Cr−C coatings (a) as-deposited, (b) annealed at 200 °C, (c) annealed at 400 °C, (d) annealed at 600 °C and Cr−C/Al2O3 composite coatings (e)
as-deposited, (f) annealed at 200 °C, (g) annealed at 400 °C, (h) annealed at 600 °C.
The dynamic micro-hardness of Cr−C coatings and Cr−C/Al2O3 composite coatings analyzed
by a nano-indentation test can be calculated using the formula developed by Oliver et al.  as follows:
(1) where H, Pmax, hc and Ac defined as the dynamic micro-hardness, the peak load, the contact depth, and contact area, respectively. α was a constant that depends on the indenter shape. In this study, α was kept at 15.08, which corresponded to the indenter with a tip angle of 100°.
Fig. 9 presents the hardness of Cr−C coatings and Cr−C/Al2O3 composite coatings annealed at
various temperatures. The hardness of samples increases with increasing of heat treatment temperature and the hardness of Cr−C/Al2O3 composite coatings is higher than that of Cr−C coatings when
annealing at same temperature. The Cr−C and Cr−C/Al2O3 composite coating exhibit the maximum
hardness of 19.42 and 22.85 GPa, respectively, at the annealing temperature of 600 °C. The likely explanation to the enhancement of microhardness of these Cr−C and Cr−C/Al2O3 composite coating is
the crystallization of Cr and the precipitation of Cr23C6, Cr7C3 and Cr2O3 phases occurs at 600 °C,
Table 2. The grain size of Cr−C coatings and Cr−C/Al2O3 composite coatings annealed at different
Crystallite size (nm)
As-plated H.T. 200 ℃ H.T. 400 ℃ H.T. 600 ℃
amorphous-like 3.1 17.9 29.6
amorphous-like 1.5 4.8 18.5
It was found that the grain size increased with increased annealing temperature. The grain size for the Cr−C coating annealed at 200 °C was 3.1 nm and increased to 17.9 nm at 400 °C and to 29.6 nm at 600 °C. In the case of Cr−C/Al2O3 composite coating the grain size for the coating annealed at
200 °C was 1.5 nm and increased to 4.8 nm at 400 °C and to 18.5 nm at 600 °C. The grain size of Cr−C/Al2O3 composite coatings is smaller than that of the relevant Cr−C coatings, this can be
attributed to the incorporation of Al2O3 particles in the coating will hinder the grain growth during heat
treatment [34,35]. According to the Halle-Petch equation  the micro-hardness varies linearly with the inverse square root of the grain diameter. This relationship indicates that the hardness increases with decreasing grain size. As mentioned above, the hardness of Cr−C/Al2O3 composite coating is
higher than that of relevant Cr−C coating, both in as plated and heat-treated conditions. The mechanisms of such strengthening are the grain refinement strengthening and the dispersion strengthening effect caused by the Al2O3 particles uniformly distributed in the Cr−C matrix.
The worn surface morphologies for as-plated and heat treated Cr−C coatings and Cr−C/Al2O3
composite coatings are presented in Fig. 10. The as-plated Cr−C coating shows typical adhesive wear morphology with large debris formed on the worn surface (Fig. 10(a)). The formation of large debris and severe adhesive wear are indicative of poor wear resistance of as-plated Cr−C coating. Fig. 10(b) presents the micrographs of worn surface of Cr−C coating after heat treated at 200 ℃. After heating at 200 ℃, Fig. 10(b) exhibits some characteristics of adhesive wear and no debris appears on the surface. As it was mentioned before, the as-deposited Cr−C coating has a hardness of 9.3 GPa and the hardness increases to14.22 GPa as the samples annealed at 200 °C. Therefore, the reduction in the adhesive wear might be attributed to the increase of hardness of the coating due to the heat treatment at 200 ℃, After annealing at 400 and 600 ℃, the mechanism moves towards abrasive wear characterized by extensive plastic deformation, deep grooves and severe disruption on worn surface as shown in Fig. 10(c) and 10(d). After heat treatment at 400 and 600 ℃, the Cr−C coatings become much harder and more brittle due to the precipitation of Cr23C6, Cr7C3 and Cr2O3. During the wear test, a part of the
composite coatings. The adhesive wear appears to be the most likely wear behavior for as-plated Cr−C/Al2O3 composite coating, as supported by only slight abrasive grooves caused by the plowing
process appears on the worn surface. Fig. 10(f) shows the worn surface of Cr−C/Al2O3 composite
coatings after heating at 200 ℃. The abrasive grooves caused by the plowing process are not found due to the hardness of composite coating increase to 16.18 GPa. Fig. 10(g) and (h) show the worn surface of Cr−C/Al2O3 composite coatings annealed at 400 and 600 ℃, respectively. The wear caused
by the effect of hard third body abrasives is evident on the worn surface of Cr−C/Al2O3 composite
coatings which is similar to that of the relevant Cr−C coatings (Fig. 10(c) and (d)). This might contribute to a significant increase in specific wear rate of coatings.
Fig. 11 shows the annealing temperature effect on friction coefficients and wear rate of the Cr−C coatings and Cr−C/Al2O3 composite coatings. It can be clearly seen from Fig. 11(a) that the
average friction coefficients of Cr−C/Al2O3 composite coatings (from 0.45 to 0.73) are lower than that
of the relevant Cr−C coatings (from 0.55 to 0.81). This can be attributed to the improvement of hardness of Cr−C coatings caused by the combine effect of grain size refining and Al2O3 particles
dispersion strengthening (Fig. 9). It leads to a decrease in the average friction coefficients between the counter ball and coatings due to the inert particles uniformly distributed in the metal matrix could restrain the growth of the alloy grains and the plastic deformation of the matrix under a loading .
Fig. 11(b) shows the annealing temperature effect on wear rate of the Cr−C coatings and Cr−C/Al2O3 composite coatings, both in as plated and heat-treated conditions. The specific wear rate
of as-plated Cr−C coatings and as-plated Cr−C/Al2O3 composite coatings is approximately at 47.49 ×
Figure 11. The effect of annealing temperature on: (a) average of friction coefficient and (b) wear rate of Cr−C coating and Cr−C/Al2O3 composite coating.
The result of wear rate indicates the incorporation of Al2O3 particles into the Cr−C matrix will
significantly enhance the wear resistance of coatings due to the Al2O3 dispersion strengthening effect
enhances the hardness of the as-deposited coating from 9.02 to 10.63 GPa (Fig. 9). The lowest specific wear rate (8.8 × 10-7 mm3/Nm) was achieved for Cr−C/Al2O3 composite coating annealed at 200℃.
The increase of annealing temperature leads to a lower specific wear resistance. When the annealing temperature increases from 400 to 600 ℃, the specific wear rate of Cr−C coating and Cr−C/Al2O3
composite coating significantly increase from 42.02 to 59.84 × 10-7 mm3/Nm and 8.8 to 37.4 × 10-7 mm3/Nm, respectively. The increased specific wear rate of coatings can be attributed to the higher hardness (over 17.42 GPa) of coatings results in the occurrence of hard third body abrasives during wear resistance test.
In the present study, the effect of heat treatment on the corrosion resistance, mechanical properties and tribological behavior between Cr−C coatings and Cr−C/Al2O3 composite coatings were
examined and compared, the following conclusions have been drawn:
(1) The incorporation of Al2O3 particles into the Cr−C matrix can reduce the internal stress.
structure was maintained for the coating after annealing at 200 ℃.
(2) The Cr−C/Al2O3 composite coatings has the best corrosion resistance (icorr = 2.84 × 10-7
A/dm2) due to a crack-free structure within Cr-C matrix.
(3) The hardness of Cr−C/Al2O3 composite coatings is higher than that of Cr−C coatings,
both in as plated and heat-treated conditions. The improvement of hardness can be attributed to the combine effect of grain size refining and Al2O3 particles dispersion strengthening. The highest
micro-hardness of Cr−C/Al2O3 composite coating (22.85 GPa) was achieved for Cr−C/Al2O3 composite
coating after annealing at 600 ℃.
(4) The codeposition of Al2O3 particles within the Cr−C deposits will significantly improve
the wear resistance of coatings and reduces the wear weight loss. The lowest specific wear rate (8.8 × 10-7 mm3/Nm) was obtained for the Cr−C/Al
2O3 composite coatings heat treated at 200 ℃.
1. S. Ghaziof, M.A. Golozar, K. Raeissi, J. Alloys Compd., 496 (2010) 164. 2. Z. Zeng, L. Wang, A. Liang, J. Zhang, Electrochim. Acta, 52 (2006) 1366.
3. F.I. Danilov, V.S. Protsenko, V.O. Gordiienko, S.C. Kwon, J.Y. Lee, Kim M., Appl. Surf. Sci., 257 (2011) 8048.
4. H. Yu, B. Chen, H. Wu, X. Sun, B. Li, Electrochim. Acta, 54 (2008) 720.
5. H.H. Sheu, C.H. Lin, S.Y. Jian, H.B. Lee, B.R. Yang, M.D. Ger, Int. J. Electrochem. Sci., 11 (2016) 7099.
6. S.C. Kwon, M. Kim, Surf. Coat. Technol., 158 (2004) 151. 7. G. Saravanan, S. Mohan, Corros. Sci., 51 (2009) 197. 8. Y.B. Song, D.T. Chin, Electrochim. Acta, 48 (2002) 349.
9. C.W. Chien, C.L. Liu, F.J. Chen, K.H. Lin, C.S. Lin, Electrochim. Acta, 72 (2012) 74.
10.S. Surviliene, A. Lisowska-Oleksiak, V. Jasulaitiene, A.C. Esuniene, Trans IMF, 83 (2005) 130. 11.Q. Feng, T. Li, H. Yue, K. Qi, F. Bai, J. Jin, Appl. Surf. Sci., 254 (2008) 2262.
12.Z. Zeng, J. Zhang, Surf. Coat. Technol., 202 (2008) 2725.
13.J.N. Balaraju, V. Ezhil Selvi, K.S. Rajam, Mater. Chem. Phys., 120 (2010) 546.
14.S. Surviliene, V. Jasulaitiene, A. Lisowska-Oleksiak, V.A. Safonov, J. Appl. Electrochem., 35 (2005) 9.
15.M.H. Sarafrazi, M. Alizadeh, J. Alloys Compd., 720 (2017) 289.
16.H.T. Wang, H.H. Sheu, M.D. Ger, K.H. Hou, Surf. Coat. Technol., 259 (2014) 268.
17.P.L. Mangonon, Principles of materials selection for engineering design. Prentice Hall, London (1998).
18.Z. Zeng, J. Zhang, Surf. Coat. Technol., 202 (2008) 2725.
19.M. Salehi Doolabi, S.K. Sadrnezhaad, D. Salehi Doolabi, M. Asadirad, International Heat Treatment and Surface Engineering, 6 (2012) 178.
20.M. Salehi Doolabi, S.K. Sadrnezhaad, D. Salehi Doolabi, Anti-Corrosion Methods and Materials, 61 (2014) 205.
21.K.H. Hou, M.C. Jeng, M.D. Ger, J. Alloys Compd., 437 (2007) 289. 22.A. Martín, J. Rodríguez, J. Llorca, Wear, 225–229 (1999) 615.
23.I. Apachitei, F.D. Tichelaar, J. Duszczyk, L. Katgerman, Surf. Coat. Technol., 149 (2002) 263. 24.A. Liang, L. Ni, Q. Liu, J. Zhang, Surf. Coat. Technol., 218 (2013) 23.
25.H.H. Sheu, C.E. Lu, K.H. Hou, M.L. Kuo, M.D. Ger, Journal of the Taiwan Institute of Chemical Engineers, 48 (2015) 73.
27.R. Furushima, K. Katou, S. Nakao, Z.M. Sun, K. Shimojima, H. Hosokawa, International Journal of Refractory Metals and Hard Materials, 42 (2014) 42.
28.C.A. Huang, W. Lin, S.C. Chen, M.C. Liao, Mater. Sci. Eng. A, 403 (2005) 222. 29.C.A. Huang, U.W. Lieu, C.H. Chuang, Surf. Coat. Technol., 203 (2009) 2921.
30.H.F. Xuan, Q.Y. Wang, S.L. Bai, Z.D. Liu, H.G. Sun, P.C. Yan, Surf. Coat. Technol., 244 (2014) 203.
31.M. Masanta, S.M. Shariff, Mater. Sci. Eng. A, 528 (2011) 5327.
32.G.F. Sun, R. Zhou, Y.K. Zhang, G.D. Yuan, K. Wang, X.D. Ren, D.P. Wen, Optics Laser Technol., 62 (2014) 20.
33.W.C. Oliver, G.M. Pharr, J. Mater. Res., 19 (2004) 3.
34.E. Budevski, G. Staikov, W.J. Lorenz, Electrochim. Acta, 45 (2000) 2559. 35.S.C. Wang, W.J. Wei, J. Mater. Res., 18 (2003) 1566.
36.N.J. Petch, Prog. Mater. Phys., 5 (1954) 1.
37.S. Mahdavi, S.R. Allahkaram, J. Alloys Compd., 635 (2015) 150. 38.Y. Yao, S. Yao, L. Zhang, H. Wang, Mater. Lett., 61 (2007) 67.